Protocolos atuais para cimentação adesiva de próteses cerâmicas

AUTORES

Rodrigo Othávio de Assunção e Souza
Professor adjunto da disciplina de Prótese Fixa – Universidade Federal do Rio Grande do Norte. Orcid: 0000-0003-0856-7178.

Nathalia Ramos da Silva
Especialista, mestra e doutora em Prótese Dentária, programa de pós-graduação em Ciências Odontológicas (área de concentração em Clínicas Odontológicas) – Universidade Federal do Rio Grande do Norte. Orcid: 0000-0003-4153-3279.

Marco Antonio Bottino
Professor titular da disciplina de Prótese Dentária – ICT-Unesp. Orcid: 0000-0003-0077-3161.

RESUMO

A etapa de cimentação adesiva de próteses cerâmicas é um ponto-chave para o seu sucesso clínico e longevidade. Com a evolução dos protocolos de cimentação e das cerâmicas, novos materiais têm surgido no mercado, o que pode gerar dúvidas sobre a escolha do método e dos materiais para a cimentação adesiva dos diferentes tipos de prótese cerâmica. Portanto, este trabalho buscou revisar a literatura atual sobre os protocolos de cimentação adesiva para próteses cerâmicas e nortear a decisão sobre o protocolo de cimentação adesiva indicado para as cerâmicas acidossensíveis ou acidorresistentes.

Palavras-chave – Cerâmica; Tratamento de superfície; Cimentação adesiva; Prótese dentária.

ABSTRACT

The adhesive cementation step of all-ceramic prostheses is a key point for their clinical success and longevity. With the evolution of cementation protocols and ceramics, new materials have appeared on the market, which can raise doubts about the choice of method and materials for adhesive cementation of different types of ceramic prostheses. Therefore, this work seeks to review the current literature on adhesive cementation protocols for all-ceramic prostheses and guide the decision on the adhesive cementation indicated for acidsensitive or acid-resistant ceramics.

Key words – Dental ceramics; Surface treatment; Adhesive cementation; Dental prosthesis.

Referências

Morimoto S, Albanesi RB, Sesma N, Agra CM, Braga MM. Main clinical outcomes of feldspathic porcelain and glass-ceramic laminate veneers: a systematic review and meta-analysis of survival and complication rates. Int J Prosthodont 2016;29(1):38-49.

Morimoto S, de Sampaio FBR, Braga MM, Sesma N, Özcan M. Survival rate of resin and ceramic inlays, onlays, and overlays: a systematic review and meta-analysis. J Dent Res 2016;95(9):985-94.

Vila-Nova TEL, Moura DMD, Araújo GM, Pinto RAS, Leite FPP, Melo RM et al. Effect of adhesive resin application on the durability of adhesion to CAD/CAM glass-ceramics after either hydrofluoric acid etching or self-etch primer application. J Adhes Dent 2022;24(1):279-89.

Lima CM, Silva NRD, Martins JD, Miranda JS, Tanaka R, Souza ROAE et al. Effect of different surface treatments on the biaxial flexure strength, Weibull characteristics, roughness, and surface topography of bonded CAD/CAM silica-based ceramics. Dent Mater 2021;37(3):151-61.

da Silva SEG, de Araújo GM, Souza KB, Moura DMD, Aurélio IL, May LG et al. Biaxial flexure strength and physicochemical characterization of a CAD/CAM lithium disilicate ceramic: effect of etching time, silane, and adhesive applications. Clin Oral Investig 2022;26(11):6753-63.

Souza ROA, Bottino MA. Cimentação adesiva em próteses cerâmicas: o que realmente eu preciso saber? PróteseNews 2018;5(5):516-31.

Souza ROA. Novos materiais restauradores livres de metal. PróteseNews 2017;4(5):554-64.

Spitznagel FA, Boldt J, Gierthmuehlen PC. CAD/CAM ceramic restorative materials for natural teeth. J Dent Res 2018;97(10):1082-91.

Souza ROA, Miyashita E. Lentes de contato cerâmicas como alternativa para correção de giroversões e diastemas em área estética. PróteseNews 2014;1(1):36-49.

Kwon SJ, Lawson NC, McLaren EE, Nejat AH, Burgess JO. Comparison of the mechanical properties of translucent zirconia and lithium disilicate. J Prosthet Dent 2018;120(1):132-7.

Moura DMD, Januário ABN, de Araújo AMM, Dal Piva AMO, Özcan M, Bottino MA et al. Effect of primer-cement systems with different functional phosphate monomers on the adhesion of zirconia to dentin. J Mech Behav Biomed Mater 2018;88:69-77.

Souza R, Barbosa F, Araújo G, Miyashita E, Bottino MA, Melo R et al. Ultrathin monolithic zirconia veneers: reality or future? Report of a clinical case and one-year follow-up. Oper Dent 2018;43(1):3-11.

Vila-Nova TEL, de Carvalho IHG, Moura DMD, Batista AUD, Zhang Y, Paskocimas CA et al. Effect of finishing/polishing techniques and low temperature degradation on the surface topography, phase transformation and flexural strength of ultra-translucent ZrO2 ceramic. Dent Mater 2020;36(4):126-39.

Carvalho IHG, da Silva NR, Vila-Nova TEL, de Almeida LFD, Veríssimo AH, de Melo RM et al. Effect of finishing/polishing techniques and aging on topography, C. albicans adherence, and flexural strength of ultra-translucent zirconia: an in situ study. Clin Oral Investig 2022;26(1):889-900.

Michailova M, Elsayed A, Fabel G, Edelhoff D, Zylla IM, Stawarczyk B. Comparison between novel strength-gradient and color-gradient multilayered zirconia using conventional and high-speed sintering. J Mech Behav Biomed Mater 2020;111:103977.

Schönhoff LM, Lümkemann N, Buser R, Hampe R, Stawarczyk B. Fatigue resistance of monolithic strength-gradient zirconia materials. J Mech Behav Biomed Mater 2021;119:104504.

Barca DC, Moura DMD, Costa GFA, Pavanelli CA, Bottino MA, Souza ROA. Influence of ceramic thickness and light-curing time on the long-term µTBS of silica-based ceramic to human dentin. J Adhes Sci Technol 2017;31(15):1700-10.

Martins JD, Moura D, Lima CM, de Carvalho R, Leite F, Souza R. Surface treatment and cementation of lithium silicate ceramics containing ZrO2. Oper Dent 2022;47(2):202-13.

Venturini AB, Prochnow C, Rambo D, Gundel A, Valandro LF. Effect of hydrofluoric acid concentration on resin adhesion to a feldspathic ceramic. J Adhes Dent 2015;17(4):313-20.

Lung CY, Matinlinna JP. Aspects of silane coupling agents and surface conditioning in dentistry: an overview. Dent Mater 2012;28(5):467-77.

Saraçoğlu A, Cura C, Cötert HS. Effect of various surface treatment methods on the bond strength of the heat-pressed ceramic samples. J Oral Rehabil 2004;31(8):790-7.

Moura DMD, Carvalho IHG, Araújo GM, Souza KB; Vila-Nova TEL, Miranda LM et al. Cimentação adesiva em cerâmicas vítreas: silanização. Parte II. PróteseNews 2019;6(6):705-8.

Vila-Nova TEL, Silva NR, Moura DMD, Araújo GM, Miranda LM, Carvalho IHG et al. Cimentação adesiva em cerâmicas vítreas. Condicionamento e limpeza pós-condicionamento. Parte I. PróteseNews 2019;6(5):587-90.

Sundfeld Neto D, Naves LZ, Costa AR, Correr AB, Consani S, Borges GA et al. The effect of hydrofluoric acid concentration on the bond strength and morphology of the surface and interface of glass ceramics to a resin cement. Oper Dent 2015;40(5):470-9.

Veríssimo AH, Moura DMD, Tribst JPM, Araújo AMM, Leite FPP, Souza ROA. Effect of hydrofluoric acid concentration and etching time on resin-bond strength to different glass ceramics. Braz Oral Res 2019;33:e041.

May MM, Fraga S, May LG. Effect of milling, fitting adjustments, and hydrofluoric acid etching on the strength and roughness of CAD-CAM glass-ceramics: a systematic review and meta-analysis. J Prosthet Dent 2022;128(6):1190-200.

Murillo-Gómez F, Palma-Dibb RG, De Goes MF. Effect of acid etching on tridimensional microstructure of etchable CAD/CAM materials. Dent Mater 2018;34(6):944-55.

Bruzi G, Carvalho AO, Giannini M, Maia HP, Magne P. Post-etching cleaning influences the resin shear bond strength to CAD/CAM lithium-disilicate ceramics. Appl Adhes Sci 2017;5(17):1-9.

Conejo J, Ozer F, Mante F, Atria PJ, Blatz MB. Effect of surface treatment and cleaning on the bond strength to polymer-infiltrated ceramic network CAD-CAM material. J Prosthet Dent 2021;126(5):698-702.

Cotes C, de Carvalho RF, Kimpara ET, Leite FP, Ozcan M. Can heat treatment procedures of pre-hydrolyzed silane replace hydrofluoric acid in the adhesion of resin cement to feldspathic ceramic? J Adhes Dent 2013;15(6):569-74.

Silva UPC, Maia AP, Silva ID, Miranda ME, Brandt WC. Influence of the multiple layers application and the heating of silane on the bond strength between lithium disilicate ceramics and resinous cement. Eur J Dent 2021;15(4):720-6.

Yoshihara K, Nagaoka N, Sonoda A, Maruo Y, Makita Y, Okihara T et al. Effectiveness and stability of silane coupling agent incorporated in ‘universal’ adhesives. Dent Mater 2016;32(10):1218-25.

Lee HY, Han GJ, Chang J, Son HH. Bonding of the silane containing multi-mode universal adhesive for lithium disilicate ceramics. Restor Dent Endod 2017;42(2):95-104.

Souza KB, Moura DMD, Silva SEGD, Araújo GM, Pinto RAS, Leite FPP et al. Effect of different surface treatments and multimode adhesive application on the Weibull characteristics, wettability, surface topography and adhesion to CAD/CAM lithium disilicate ceramic. J Appl Oral Sci 2020;28:e20200122.

Passos SP, Valandro LF, Amaral R, Ozcan M, Bottino MA, Kimpara ET. Does adhesive resin application contribute to resin bond durability on etched and silanized feldspathic ceramic? J Adhes Dent 2008;10(6):455-60.

Araújo AMM, Januário ABDN, Moura DMD, Tribst JPM, Özcan M, Souza ROA. Can the application of multi-mode adhesive be a substitute to silicatized/silanized Y-TZP ceramics? Braz Dent J 2018;29(3):275-81.

Nogueira IO, Oliveira PFG, Magno MB, Ferreira DMTP, Maia LC, Rabello TB. Does the application of an adhesive layer improve the bond strength of etched and silanized glass-ceramics to resin-based materials? A systematic review and meta-analysis. J Prosthet Dent 2021;125(1):56-64.

Tribst J, Anami LC, Özcan M, Bottino MA, Melo RM, Saavedra G. Self-etching primers vs acid conditioning: impact on bond strength between ceramics and resin cement. Oper Dent 2018;43(4):372-9.

Souza R, da Silva NR, de Miranda LM, de Araújo GM, Moura D, Barbosa H. Two-year follow-up of ceramic veneers and a full crown treated with self-etching ceramic primer: a case report. Oper Dent 2020;45(4):352-8.

Lyann SK, Takagaki T, Nikaido T, Wada T, Uo M, Ikeda M et al. Efficacy of various surface treatments on the bonding performance of saliva-contaminated lithium-disilicate ceramics. J Adhes Dent 2019;21(1):51-8.

Yoshida K. Influence of cleaning methods on the bond strength of resin cement to saliva-contaminated lithium disilicate ceramic. Clin Oral Investig 2020;24(6):2091-7.

Fagan J, Vesselovcz J, Puppin-Rontani J, Correr-Sobrinho L, Freitas K, Robertson TC et al. Evaluation of cleaning methods on lithium disilicate glass ceramic surfaces after organic contamination. Oper Dent 2022;47(2):E81-E90.

Pereira LL, Campos F, Dal Piva AM, Gondim LD, Souza RO, Özcan M. Can application of universal primers alone be a substitute for airborne-particle abrasion to improve adhesion of resin cement to zirconia? J Adhes Dent 2015;17(2):169-74.

Alves M, Campos F, Bergoli CD, Bottino MA, Özcan M, Souza R. Effect of adhesive cementation strategies on the bonding of Y-TZP to human dentin. Oper Dent 2016;41(3):276-83.

Aboushelib MN, Kleverlaan CJ, Feilzer AJ. Selective infiltration-etching technique for a strong and durable bond of resin cements to zirconia-based materials. J Prosthet Dent 2007;98(5):379-88.

Bottino MA, Bergoli C, Lima EG, Marocho SM, Souza RO, Valandro LF. Bonding of Y-TZP to dentin: effects of Y-TZP surface conditioning, resin cement type, and aging. Oper Dent 2014;39(3):291-300.

Campos TM, Ramos NC, Machado JP, Bottino MA, Souza RO, Melo RM. A new silica-infiltrated Y-TZP obtained by the sol-gel method. J Dent 2016;48:55-61.

Campos TMB, Ramos NC, Matos JDM, Thim GP, Souza ROA, Bottino MA et al. Silica infiltration in partially stabilized zirconia: effect of hydrothermal aging on mechanical properties. J Mech Behav Biomed Mater 2020;109:103774.

Queiroz JRC, Duarte DA, Souza ROA, Fissmer SF, Massi M, Bottino MA. Deposition of SiOx thin films on Y-TZP by reactive magnetron sputtering: influence of plasma parameters on the adhesion properties between Y-TZP and resin cement for application in dental prosthesis. Mat Res 2011;14(2):212-6.

Melo RM, Souza RO, Dursun E, Monteiro EB, Valandro LF, Bottino MA. Surface treatments of zirconia to enhance bonding durability. Oper Dent 2015;40(6):636-43.

Ramos NC, Alves LMM, Ramos GF, Bottino MA, Melo RM, Souza ROA. The importance of MDP priming, silica blasting or glazing on the retention force of Y-TZP copings to varying geometry tooth abutments. Coatings 2021;11(3):315.

Özcan M, Bernasconi M. Adhesion to zirconia used for dental restorations: a systematic review and meta-analysis. J Adhes Dent 2015;17(1):7-26.

Araújo GM, Vila-Nova TEL, Moura DMD, Araújo LMM, Ferreira JV, Gurgel BCV et al. Lentes de contato em zircônia monolítica ultratranslúcida: realidade ou futuro? Relato de caso com um ano de acompanhamento clínico. PróteseNews 2018;5(4):414-24.

Quigley NP, Loo DSS, Choy C, Ha WN. Clinical efficacy of methods for bonding to zirconia: a systematic review. J Prosthet Dent 2021;125(2):231-40.

Silva NRD, Araújo GM, Vila-Nova TEL, Bezerra MGPG, Calderon PDS, Özcan M et al. Which zirconia surface-cleaning strategy improves adhesion of resin composite cement after saliva contamination? A systematic review and meta-analysis. J Adhes Dent 2022;24(1):175-86.

Scholz KJ, Tabenski IM, Vogl V, Cieplik F, Schmalz G, Buchalla W et al. Randomized clinical split-mouth study on the performance of CAD/CAM-partial ceramic crowns luted with a self-adhesive resin cement or a universal adhesive and a conventional resin cement after 39 months. J Dent 2021;115:103837.

Miotti LL, Follak AC, Montagner AF, Pozzobon RT, da Silveira BL, Susin AH. Is conventional resin cement adhesive performance to dentin better than self-adhesive? A systematic review and meta-analysis of laboratory studies. Oper Dent 2020;45(5):484-95.